Statement of Problem There are limited studies evaluating the effect of a cyclic load on interim fixed prosthetic materials and its effect on flexural strength
Purpose of Study (1) To verify the flexural strength of previously studied interim fixed prosthetic materials. (2) To establish the flexural strength of new, advanced generation and untested interim fixed prosthetic materials. (3) To determine the effect of cyclic load on the flexural strength of interim fixed prosthetic materials
Materials and Methods. Bar-type specimens of Caulk Temporary Bridge Resin, VitaVM CC, Protemp 3 Garant and Radica were fabricated according to International Standards Organization 4049 and American National Standards Institute/American Dental Association specification 27. After being stored in distilled water for 10 days, specimens were divided into Noncycled and Cycled Groups. The Noncycled Group specimens were fractured under a 3-point loading in a Bose Electroforce 3300 testing instrument at a crosshead speed of 0.75 mm/min. Cycled Groups specimens underwent a 6-12 Newton 3 Hertz cyclic load for 20,000 cycles in a Bose Electroforce 3300 testing instrument. Immediately following completion of the cycles, the specimens were fractured under a 3-point loading. Maximal loads to fracture in Newtons were recorded and mean flexural strengths were calculated (n = 20 per group). Comparisons were made with analysis of variance and Tukey's Multiple Comparison Test
Results. Noncycled (NC) and Cycled (C) groups order of mean flexural strengths (MPa) from lowest to highest mean were as follows: Caulk (Noncycled - 53.83; C - 60.02), Vita VM CC (NC - 65.96; C - 66.83), Protemp 3 Garant (NC - 75.85; C - 77.18), and Radica (NC - 106.1; C - 115.96). In the Noncycled and Cycled groups, Radica was statistically superior when compared to all materials and Protemp 3 Garant was statistically superior to Caulk Temporary Bridge Resin. There was no statistically significant difference between the material's flexural strengths before and after cycles.
Conclusion. Within the limitations of this study, 20,000 cyclic loads of 6-12 Newtons at 3 Hertz did not have a significant effect on the flexural strength of interim fixed prosthetic materials. Radica demonstrated significantly superior flexural strength over other materials tested.
|Advisor:||Gratton, David G.|
|Commitee:||Diaz-Arnold, Ana M., Schneider, Galen B., Vargas, Marcos A.|
|School:||The University of Iowa|
|School Location:||United States -- Iowa|
|Source:||MAI 48/03M, Masters Abstracts International|
|Keywords:||Flexural strength, Interim fixed prosthesis|
Copyright in each Dissertation and Thesis is retained by the author. All Rights Reserved
The supplemental file or files you are about to download were provided to ProQuest by the author as part of a
dissertation or thesis. The supplemental files are provided "AS IS" without warranty. ProQuest is not responsible for the
content, format or impact on the supplemental file(s) on our system. in some cases, the file type may be unknown or
may be a .exe file. We recommend caution as you open such files.
Copyright of the original materials contained in the supplemental file is retained by the author and your access to the
supplemental files is subject to the ProQuest Terms and Conditions of use.
Depending on the size of the file(s) you are downloading, the system may take some time to download them. Please be